# TOPIC 2. STRUCTURE OF MATERIALS III

Save this PDF as:

Size: px
Start display at page:

Download "TOPIC 2. STRUCTURE OF MATERIALS III"

## Transcription

1 Universidad Carlos III de Madrid MATERIALS SCIENCE AND ENGINEERING TOPIC 2. STRUCTURE OF MATERIALS III Topic 2.3: Crystalline defects. Solid solutions. 1

2 PERFECT AND IMPERFECT CRYSTALS Perfect crystal: All the atoms are in the ideal lattice positions (only true at 0 K). Real crystal: atoms vibrate - There positions that are not occupied (vacancies) - atoms displaced from ideal positions - There are defects that modify the properties 2

3 PERFECT AND IMPERFECT CRYSTALS Thermodynamics Justify of defects, as ΔG crystal Creation of a defect ΔH > 0 and ΔS > 0 Configuration Entropy S = k B ln W K B = Boltzmann constant = JK -1 W=way of distributing n defects in N possible positions arbitrarily In 1 mol of C + there are N A possibilities to create 1 vacancy W When T [defects] Vacancy or defect: ΔH<TΔS ΔG= ΔH-TΔS<0 3

4 DEFECTS TYPES (according to dimensions) 1. Point : Vacancies Interstitials Substitutional Schottky Frenkel Order-Disorder 2. Linear: dislocations: Edge Screw Mixed 3. Complex: clusters 4. Planar or Extended External Surfaces Grain Boundaries Twin Boundaries Stacking Faults 4

5 POINT DEFECTS: VACANCIES AND INTERSTITIALS Vacancy: When an atom is missing from a position where it should be. Interstitial: An atom from the crystal occupies the place of an interstitial (self-interstitial or interstitialcy) n v = nº vacancies per cm 3 N= nº of lattice points per cm 3 n v /N = fraction of vacancies ΔH v = Formation energy (J.mol -1 ) vacancies concentration at equilibrium They are produced : during solidification (impurities, alloys) by particle bombardment with E during plastic deformation (processing) when T thermal vibrations n v 5

6 POINT DEFECTS: SCHOTTKY AND FRENKEL DEFECTS IN IONIC CRYSTALS Schottky Defect: Vacancy in an ionic crystal. In order to maintain neutrality Anionic and cationic vacancies appear Frenkel Defect: migration of an ion from its normal position to an interstitial position (combination vacancy-interstitial) 6

7 POINT DEFECTS: SCHOTTKY AND FRENKEL Nº of Schottky defects: n s Nº of Frenkel defects : n F ΔH S = E for Schottky defect creation ΔH F = E for Frenkel defect creation N= nº of lattice positions N i = nº of interstitial positions T= Temperature (K) In a crystal ΔH S ΔH F the defect with the lowest ΔH will form nº defects increases with temperature 7

8 POINT DEFECTS: SCHOTTKY AND FRENKEL Compound ΔH (ev) ΔH (10-19 J) Schottky defects MgO CaO LiF LiCl NaCl KCl Frenkel defects ZrO CaF SrF AgCl AgBr NaCl (T f =801 ºC) ΔH s = 3.69x10-19 J T=300K n s = 2.64x10 4 vacancies/mol T=1000K n s = 9.38x10 17 vacancies/mol MgO ΔH s = 10.57x10-19 J T=300K n s = 2.12x10-32 vacancies/mol T=1000K n s = 1.39x10 7 vacancies/mol ΔH s (MgO) > ΔH s (NaCl) n s low, more difficult to create vacancies. 8

9 POINT DEFECTS: ORDER-DISORDER IN SOLID SOLUTIONS Order-disorder phenomena (in substitutional solid solutions): Atoms of one sub-lattice occupy positions corresponding to the other and vice versa (metallic alloys). Solids with elements that have similar electronegativity β' 450 ºC Cu/Zn β (bcc) T>390 ºC Disordered T<390 ºC Ordered Zn Cu or vice versa Brass β (ordered) Brass β : Cu centre Zn corners average gold-copper atom copper atom gold atom Cu-Au Alloys Brass β: Cu and Zn arbitrarily distributed in BCC 9

10 LINEAR DEFECTS : DISLOCATIONS DISLOCATIONS They are defects that produce distortion in the lattice situated around a line. Characteristics: they can be displaced in the interior of a crystal by applying relatively low forces and can produce a complete displacement over crystalline planes. Explain: - E theoretical ( Young modulus) > E experimental - Plastic deformation in metals (workability, ductility) Formation: - during solidification - through plastic or permanent deformation of crystal - through concentration of vacancies - through atomic disarrangements in solid solutions Types: - edge dislocation, or Taylor dislocation - screw dislocation, or Burgers dislocation - mixed dislocation 10

11 EDGE DISLOCATIONS (or TAYLOR) Geometric modification of the lattice: equivalent to an extra plane of atoms Energetic modification (they store energy) Direction of motion Dislocation line.- point A Slipping plane.- line of points William D. Callister, Jr., Materials Science and Engineering : An Introduction, John Wiley & Sons, Inc. 11

12 EDGE DISLOCATIONS (or TAYLOR) * Dislocation characterization: Burgers Vector (b) Burgers Vector: magnitude and direction of the lattice distortion associated with the dislocation Magnitude: distance 1-5 Direction: 1-5 or 5-1 b to dislocation line b to the direction movement 12

13 SCREW DISLOCATIONS (or BURGER) Locally curves some atom lines. The effect is as if a shear stress is applied to produce a distortion Direction of motion We can move from the inferior to the superior plane through the dislocation line. William D. Callister, Jr., Materials Science and Engineering : An Introduction, John Wiley & Sons, Inc. 13

14 SCREW DISLOCATIONS (or BURGER) * Burgers Vectors in screw dislocations: The magnitude and distance from 1-5 define b b to dislocation line SS b to the direction of movement We can trace a screw (spiral ramp) around the dislocation. dislocation line

15 MIXED DISLOCATIONS If there are many dislocations they are mixed ( MIXED dislocations) Screw Edge Burgers Vector = b The Burgers vector will be the same at all points along its line even though the dislocation might change direction and nature within a crystal. William D. Callister, Jr., Materials Science and Engineering : An Introduction, John Wiley & Sons, Inc. 15

16 DISLOCATIONS MOVEMENT Dislocation movement (edge and screw) when a shear stress is applied Slip direction Slip plane slip direction: the direction in which the dislocation moves slip plane: the plane in which the dislocation moves The combination of the slip direction and the slip plane is the slip system 16

17 PLASTIC DEFORMATION : SLIPPING OF DISLOCATIONS Dislocations movement parallel to the directions of maximum packing Lower distance between them + easy sliping Compact Direction E used to move a dislocation= E b 2 For metallic materials, the burgers vector for a dislocation will be the magnitude equal to the interatomic spacing. b = 2R E b 4R 2 NON Compact Direction E b 8R 2 A.R. West. Solid State Chemistry and its applications. Wiley.Chichester,

18 PLANAR DEFECTS: GRAIN BOUNDARIES They separate crystals with different orientation. Formation: during solidification: crystals are formed when nuclei grow simultaneously. Grain boundary They limit dislocations movement in the material 18

19 PLANAR DEFECTS : GRAIN BOUNDARIES Boundary width: 2-5 interatomic distances Very energetic zones (atomic packing < less than in interior ): - Solid state reactions - Atomic diffusion Materials properties = f (grain size) When grain size Mechanical resistance Dislocation movement is limited when there are many grain boundaries. William D. Callister, Jr., Materials Science and Engineering : An Introduction, John Wiley & Sons, Inc. 19

20 PLANAR DEFECTS: EXTERNAL SURFACES EXTERNAL SURFACE It is the end of the crystal or grain structure Coordination numbers at the surface < at the interior of the crystal E surface > E interior 20

21 PLANAR DEFECTS : STACKING FAULTS STACKING FAULTS In fcc and hcp structures hcp fcc perfect lattice :...ABABAB......ABCABCABC... Stacking fault:...ababcab......abcababc... 21

22 PLANAR DEFECTS : TWIN BOUNDARIES Twin boundary: Boundary that separates two parts of a crystal with a small difference in the orientation (misorientation) of the planes (crystal twinning). Highly symmetrical interface, often with one crystal the mirror image of the other Formation: Deformation process or during thermal treatments *Produce mechanical resistance make difficult dislocation gliding Twin boundary 22

23 PLANAR DEFECTS: TWIN BOUNDARIES Brass (70 Cu / 30 Zn) 23

24 SOLID SOLUTION 24

25 SOLID SOLUTION A) Substitutional solid solution B) Interstitial solid solution T>T f during cooling 70g Cu (fcc) + 30 g Ni (fcc) in liquid state new structure with a intermediate between Cu and Ni Small atoms located in octahedral sites or tetrahedral sites Ni Cu 25

26 SOLID SOLUTION : HUME-ROTHERY RULES Hume-Rothery rules for the formation of substitutional solid solutions : 1) The same crystal structure 2) Atoms or ions with similar radius For ceramics difference < 30% For metals difference < 15% For differences > 15% limited solubility (<1%) 5) They must have similar electronegativities 6) Valance: In ceramics: They must have the same valance. If all conditions are fulfilled we do not necessarily have total solubility -If one or more conditions are not fulfilled partial solubility 26

### Defects and Diffusion

Defects and Diffusion Goals for the Unit Recognize various imperfections in crystals Point imperfections Impurities Line, surface and bulk imperfections Define various diffusion mechanisms Identify factors

More information

### Point Defects. Vacancies are the most important form. Vacancies Self-interstitials

Grain Boundaries 1 Point Defects 2 Point Defects A Point Defect is a crystalline defect associated with one or, at most, several atomic sites. These are defects at a single atom position. Vacancies Self-interstitials

More information

### Chapter Outline Dislocations and Strengthening Mechanisms. Introduction

Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip

More information

### CRYSTAL STRUCTURE, MECHANICAL BEHAVIOUR & FAILURE OF MATERIALS

MODULE ONE CRYSTAL STRUCTURE, MECHANICAL BEHAVIOUR & FAILURE OF MATERIALS CRYSTAL STRUCTURE Metallic crystal structures; BCC, FCC and HCP Coordination number and Atomic Packing Factor (APF) Crystal imperfections:

More information

### Chapter 12: Structures & Properties of Ceramics

Chapter 12: Structures & Properties of Ceramics ISSUES TO ADDRESS... Review of structures for ceramics How are impurities accommodated in the ceramic lattice? In what ways are ceramic phase diagrams similar

More information

### Point Defects in Metals

CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Point Defects in Metals 5.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 327 C (600 K). Assume an energy

More information

### Dislocations and Plastic Deformation

Dislocations and Plastic Deformation Edge and screw are the two fundamental dislocation types. In an edge dislocation, localized lattice distortion exists along the end of an extra half-plane of atoms,

More information

### CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS

CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and Self-Interstitials 5.1 Calculate the fraction of atom sites that are vacant for copper at its melting temperature of 1084 C (1357 K). Assume

More information

### Point Defects LATTICE VACANCIES 585. DIFFUSION 588 Metals 591. COLOR CENTERS 592 F centers 592 Other centers in alkali halides 593 PROBLEMS 595

ch20.qxd 9/22/04 5:27 PM Page 583 20 Point Defects LATTICE VACANCIES 585 DIFFUSION 588 Metals 591 COLOR CENTERS 592 F centers 592 Other centers in alkali halides 593 PROBLEMS 595 1. Frenkel defects 595

More information

### Impurities in Solids. Crystal Electro- Element R% Structure negativity Valence

4-4 Impurities in Solids 4.4 In this problem we are asked to cite which of the elements listed form with Ni the three possible solid solution types. For complete substitutional solubility the following

More information

### C h a p t e r 4 : D e f e c t s i n C r y s t a l s

C h a p t e r 4 : D e f e c t s i n C r y s t a l s...perfection's a gift of The gods, few can boast they possess it - and most Of you, my dears, don't. - Ovid, The Art of Love Chapter 4: Defects in Crystals...

More information

### 3. Anisotropic blurring by dislocations

Dynamical Simulation of EBSD Patterns of Imperfect Crystals 1 G. Nolze 1, A. Winkelmann 2 1 Federal Institute for Materials Research and Testing (BAM), Berlin, Germany 2 Max-Planck- Institute of Microstructure

More information

### Module-6. Dislocations and Strengthening Mechanisms

Module-6 Dislocations and Strengthening Mechanisms Contents 1) Dislocations & Plastic deformation and Mechanisms of plastic deformation in metals 2) Strengthening mechanisms in metals 3) Recovery, Recrystallization

More information

### CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS ev /atom = exp. kt ( =

CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and Self-Interstitials 5.1 Calculate the fraction of atom sites that are vacant for copper at its melting temperature of 1084 C (1357 K). Assume

More information

### Packing of atoms in solids

MME131: Lecture 6 Packing of atoms in solids A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s topics Atomic arrangements in solids Points, directions and planes in unit cell References:

More information

### Objective To study the time and temperature variations in the hardness of Al-4% Cu alloy on isothermal aging.

EXPERIMENT 8 PRECIPITATION HARDENING IN 2024 ALUMINUM Objective To study the time and temperature variations in the hardness of Al-4% Cu alloy on isothermal aging. Introduction Materials can be hardened

More information

### Definition and description of different diffusion terms

Definition and description of different diffusion terms efore proceeding further, it is necessary to introduce different terms frequently used in diffusion studies. Many terms will be introduced, which

More information

### 1. Use the Ellingham Diagram (reproduced here as Figure 0.1) to answer the following.

315 Problems 1. Use the Ellingham Diagram (reproduced here as Figure 0.1) to answer the following. (a) Find the temperature and partial pressure of O 2 where Ni(s), Ni(l), and NiO(s) are in equilibrium.

More information

### Ph.D. Admission 20XX-XX Semester X

Ph.D. Admission 20XX-XX Semester X Written Examination Materials Science & Engineering Department, IIT Kanpur Date of Examination: XX XXXX 20XX Timing: XX:XX XX:XX XX Application# Please read these instructions

More information

### Chapter Outline How do atoms arrange themselves to form solids?

Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Face-centered cubic Body-centered cubic Hexagonal close-packed Close packed

More information

### The Structure of Materials

The Structure of Materials Samuel M. Allen Edwin L. Thomas Massachusetts Institute of Technology Cambridge, Massachusetts / John Wiley & Sons, Inc. New York Chichester Weinheim Brisbane Singapore Toronto

More information

### Planar Defects in Materials. Planar Defects in Materials

Classification of Defects in Solids: Planar defects: Stacking faults o {311} defects in Si o Inversion domain boundaries o Antiphase boundaries (e.g., super dislocations): analogous to partials but in

More information

### Unit 1 The Solid State

Points to Remember Amorphous and Crystalline Solids Unit 1 The Solid State Amorphous- short range order, Irregular shape eg-glass Crystalline Solids- long range order, regular shape eg : NaCl Molecular

More information

### Material Science. Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore India

Material Science Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore 560012 India Chapter 5. Diffusion Learning objectives: - To know the

More information

### Short-Circuit Diffusion L6 11/14/06

Short-Circuit Diffusion in Crystals 1 Today s topics: Diffusion spectrum in defective crystals Dislocation core structure and dislocation short circuits Grain boundary structure Grain boundary diffusion

More information

### Free Electron Model What kind of interactions hold metal atoms together? How does this explain high electrical and thermal conductivity?

Electrical Good conductors of heat & electricity Create semiconductors Oxides are basic ionic solids Aqueous cations (positive charge, Lewis acids) Reactivity increases downwards in family Mechanical Lustrous

More information

### 3.40 Sketch within a cubic unit cell the following planes: (a) (01 1 ) (b) (112 ) (c) (102 ) (d) (13 1) Solution

3.40 Sketch within a cubic unit cell the following planes: (a) (01 1 ) (b) (11 ) (c) (10 ) (d) (13 1) The planes called for are plotted in the cubic unit cells shown below. 3.41 Determine the Miller indices

More information

### Kinetics. Rate of change in response to thermodynamic forces

Kinetics Rate of change in response to thermodynamic forces Deviation from local equilibrium continuous change T heat flow temperature changes µ atom flow composition changes Deviation from global equilibrium

More information

### Foundations of Materials Science and Engineering Lecture Note 4

Foundations of Materials Science and Engineering Lecture Note 4 April 2, 2013 Kwang Kim Yonsei University kbkim@yonsei.ac.kr 39 8 7 34 53 Y O N Se I 88.91 16.00 14.01 78.96 126.9 Solidification of Metals

More information

### Twins & Dislocations in HCP Textbook & Paper Reviews. Cindy Smith

Twins & Dislocations in HCP Textbook & Paper Reviews Cindy Smith Motivation Review: Outline Crystal lattices (fcc, bcc, hcp) Fcc vs. hcp stacking sequences Cubic {hkl} naming Hcp {hkil} naming Twinning

More information

### STATE OF SOLIDIFICATION & CRYSTAL STRUCTURE

STATE OF SOLIDIFICATION & CRYSTAL STRUCTURE Chapter Outline Determination of crystal properties or properties of crystalline materials. Crystal Geometry! Crystal Directions! Linear Density of atoms! Crystal

More information

### STRENGTHENING MECHANISM IN METALS

Background Knowledge Yield Strength STRENGTHENING MECHANISM IN METALS Metals yield when dislocations start to move (slip). Yield means permanently change shape. Slip Systems Slip plane: the plane on which

More information

### Density Computations

CHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS Fundamental Concepts 3.1 What is the difference between atomic structure and crystal structure? Unit Cells Metallic Crystal Structures 3.2 If the atomic radius

More information

### Free Electron Model What kind of interactions hold metal atoms together? How does this explain high electrical and thermal conductivity?

Electrical Good conductors of heat & electricity Create semiconductors Oxides are basic ionic solids Aqueous cations (positive charge, Lewis acids) Reactivity increases downwards in family Free Electron

More information

### 1.10 Close packed structures cubic and hexagonal close packing

1.9 Description of crystal structures The most common way for describing crystal structure is to refer the structure to the unit cell. The structure is given by the size and shape of the cell and the position

More information

### A DISLOCATION MODEL FOR THE PLASTIC DEFORMATION OF FCC METALS AN ANALYSIS OF PURE COPPER AND AUSTENITIC STEEL

A DISLOCATION MODEL FOR THE PLASTIC DEFORMATION OF FCC METALS AN ANALYSIS OF PURE COPPER AND AUSTENITIC STEEL Background In the bcc model for work hardening in single phase materials, see (6), it is assumed

More information

### Introduction to Engineering Materials ENGR2000 Chapter 3: The Structure of Crystalline Solids. Dr. Coates

Introduction to Engineering Materials ENGR2000 Chapter 3: The Structure of Crystalline Solids Dr. Coates Learning Objectives I 1. Describe difference in atomic/molecular structure between crystalline/noncrystalline

More information

### but T m (Sn0.62Pb0.38) = 183 C, so this is a common soldering alloy.

T m (Sn) = 232 C, T m (Pb) = 327 C but T m (Sn0.62Pb0.38) = 183 C, so this is a common soldering alloy. T m (Au) = 1064 C, T m (Si) = 2550 C but T m (Au0.97Si0.03) = 363 C, so thin layer of gold is used

More information

### ENGINEERING MATERIALS LECTURE #4

ENGINEERING MATERIALS LECTURE #4 Chapter 3: The Structure of Crystalline Solids Topics to Cover What is the difference in atomic arrangement between crystalline and noncrystalline solids? What features

More information

### The University of Jordan School of Engineering Chemical Engineering Department

The University of Jordan School of Engineering Chemical Engineering Department 0905351 Engineering Materials Science Second Semester 2016/2017 Course Catalog 3 Credit hours.all engineering structures and

More information

### Non-crystalline Materials

Noncrystalline (or amorphous) solids by definition means atoms are stacked in irregular, random patterns. The general term for non-crystallline solids with compositions comparable to those of crystalline

More information

### Problem 1: (a) Describe the ß-ZnS structure and show how it is related to the FCC structure.

Note: I ve finished correcting mistakes from some of the later exams but not the earlier ones. If you see a mistake, plz msg me on AIM:huangnankun or huangnankun@berkeley.edu, I ll update this document

More information

### Formability and Crystallographic Texture in Novel Magnesium Alloys

Formability and Crystallographic Texture in Novel Magnesium Alloys Carlos Soto, Dr. Pnina Ari-Gur, Andreas, Quojo Quainoo, Dr. Betsy Aller, Dr. Andrew Kline Western Michigan University Abstract By looking

More information

### Effect of Stacking Fault Energy on Evolution of Recrystallization Textures in Drawn Wires and Rolled Sheets

Materials Science Forum Vols. 495-497 (2005) pp. 1243-1248 online at http://www.scientific.net 2005 Trans Tech Publications, Switzerland 194 Effect of Stacking Fault Energy on Evolution of Recrystallization

More information

### Fundamental concepts and language Unit cells Crystal structures! Face-centered cubic! Body-centered cubic! Hexagonal close-packed Close packed

Fundamental concepts and language Unit cells Crystal structures! Face-centered cubic! Body-centered cubic! Hexagonal close-packed Close packed crystal structures Density computations Crystal structure

More information

### Chapter 10: Phase Transformations

Chapter 10: Phase Transformations ISSUES TO ADDRESS... Transforming one phase into another takes time. Fe C FCC g (Austenite) Eutectoid transformation Fe 3 C (cementite) + a (ferrite) (BCC) How does the

More information

### Lectures on: Introduction to and fundamentals of discrete dislocations and dislocation dynamics. Theoretical concepts and computational methods

Lectures on: Introduction to and fundamentals of discrete dislocations and dislocation dynamics. Theoretical concepts and computational methods Hussein M. Zbib School of Mechanical and Materials Engineering

More information

### a. 50% fine pearlite, 12.5% bainite, 37.5% martensite. 590 C for 5 seconds, 350 C for 50 seconds, cool to room temperature.

Final Exam Wednesday, March 21, noon to 3:00 pm (160 points total) 1. TTT Diagrams A U.S. steel producer has four quench baths, used to quench plates of eutectoid steel to 700 C, 590 C, 350 C, and 22 C

More information

### Alloys GENERAL CONSIDERATIONS 621 SUBSTITUTIONAL SOLID SOLUTIONS HUME-ROTHERY RULES 624

ch22.qxd 9/22/4 5:29 PM Page 619 22 Alloys GENERAL CONSIDERATIONS 621 SUBSTITUTIONAL SOLID SOLUTIONS HUME-ROTHERY RULES 624 ORDER-DISORDER TRANSFORMATION 627 Elementary theory of order 629 PHASE DIAGRAMS

More information

### Chem 241. Lecture 19. UMass Amherst Biochemistry... Teaching Initiative

Chem 241 Lecture 19 UMass Amherst Biochemistry... Teaching Initiative Announcement March 26 Second Exam Recap Water Redox Comp/Disproportionation Latimer Diagram Frost Diagram Pourbaix Diagram... 2 Ellingham

More information

### CHAPTER 3: CRYSTAL STRUCTURES & PROPERTIES

CHAPTER 3: CRYSTAL STRUCTURES & PROPERTIES ISSUES TO ADDRESS... How do atoms assemble into solid structures? (for now, focus on metals) How does the density of a material depend on its structure? When

More information

### Crystal Structures of Interest

rystal Structures of Interest Elemental solids: Face-centered cubic (fcc) Hexagonal close-packed (hcp) ody-centered cubic (bcc) Diamond cubic (dc) inary compounds Fcc-based (u 3 u,nal, ß-ZnS) Hcp-based

More information

### Chapter 10: Phase Diagrams

hapter 10: Phase Diagrams Show figures 10-1 and 10-3, and discuss the difference between a component and a phase. A component is a distinct chemical entity, such as u, Ni, NiO or MgO. A phase is a chemically

More information

### Metals I. Anne Mertens

"MECA0139-1: Techniques "MECA0462-2 additives : et Materials 3D printing", Selection", ULg, 19/09/2017 25/10/2016 Metals I Anne Mertens Introduction Outline Metallic materials Materials Selection: case

More information

### The local atomic packing of a single-component glass is quasi-crystalline

The local atomic packing of a single-component glass is quasi-crystalline Farid F. Abraham IBM Almaden Research Center San Jose, CA *Contact Address 865 Paullus Drive Hollister CA 95023 fadlow@outlook.com

More information

### J = D C A C B x A x B + D C A C. = x A kg /m 2

1. (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. (a) With vacancy diffusion, atomic

More information

### Chapter Outline: Failure

Chapter Outline: Failure How do Materials Break? Ductile vs. brittle fracture Principles of fracture mechanics Stress concentration Impact fracture testing Fatigue (cyclic stresses) Cyclic stresses, the

More information

### Recrystallization Theoretical & Practical Aspects

Theoretical & Practical Aspects 27-301, Microstructure & Properties I Fall 2006 Supplemental Lecture A.D. Rollett, M. De Graef Materials Science & Engineering Carnegie Mellon University 1 Objectives The

More information

### Ceramic Science 4RO3. Lecture 2. Tannaz Javadi. September 16, 2013

Ceramic Science 4RO3 Lecture 2 September 16, 2013 Tannaz Javadi Rule 5: In an Ionic structure the chemical environment (cations) that is surrounding an anion should be at least uniform and similar. Although

More information

### The Plastic Regime. Processes in Structural Geology & Tectonics. Ben van der Pluijm. WW Norton+Authors, unless noted otherwise 3/4/ :11

The Plastic Regime Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 3/4/2017 17:11 We Discuss The Plastic Regime Strain rate Viscosity Crystal defects

More information

### Lecture 11. Ductile Deformation and Microstructures. Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm

Lecture 11 Ductile Deformation and Microstructures Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm Crustal Fault Model EarthStructure (2 nd ed) 2 Brittle

More information

### Intrinsic Defects in Semiconductors

Intrinsic Defects in Semiconductors In all previous consideration of crystal structure and crystal growth, for simplicity it has been assumed that the silicon crystal lattice is entirely free of defects.

More information

### Phase Transformations in Metals Tuesday, December 24, 2013 Dr. Mohammad Suliman Abuhaiba, PE 1

Ferrite - BCC Martensite - BCT Fe 3 C (cementite)- orthorhombic Austenite - FCC Chapter 10 Phase Transformations in Metals Tuesday, December 24, 2013 Dr. Mohammad Suliman Abuhaiba, PE 1 Why do we study

More information

### 7.3 Bonding in Metals > Chapter 7 Ionic and Metallic Bonding. 7.3 Bonding in Metals. 7.1 Ions 7.2 Ionic Bonds and Ionic Compounds

Chapter 7 Ionic and Metallic Bonding 7.1 Ions 7.2 Ionic Bonds and Ionic Compounds 7.3 Bonding in Metals 1 Copyright Pearson Education, Inc., or its affiliates. All Rights Reserved. CHEMISTRY & YOU What

More information

### Donald Neamen 물리전자 / 김삼동 1-1

An Introduction to Semiconductor Devices Donald Neamen Images and illustrations from supplements of An Introduction to Semiconductor Devices, 4 th Ed., Mc Graw Hill were used for this lecture materials.

More information

### Lectures on: Introduction to and fundamentals of discrete dislocations and dislocation dynamics. Theoretical concepts and computational methods

Lectures on: Introduction to and fundamentals of discrete dislocations and dislocation dynamics. Theoretical concepts and computational methods Hussein M. Zi School of Mechanical and Materials Engineering

More information

### STRUCTURE OF MATERIALS The Key to its Properties A Multiscale Perspective

STRUCTURE OF MATERIALS The Key to its Properties A Multiscale Perspective Anandh Subramaniam Materials and Metallurgical Engineering INDIAN INSTITUTE OF TECHNOLOGY KANPUR Kanpur- 208016 Email: anandh@iitk.ac.in

More information

### Physics of Nanomaterials. Module II. Properties of Nanomaterials. Learning objectives

Physics of Nanomaterials Module II Properties of Nanomaterials Learning objectives Microstructure and defects in nanomaterials, dislocations, twins, stacking faults and voids, grain boundaries Effect of

More information

### TENSION/COMPRESSION ASYMMETRY IN CREEP BEHAVIOR OF A Ni-BASED SUPERALLOY

Pergamon Scripta Materialia, Vol. 41, No. 5, pp. 461 465, 1999 Elsevier Science Ltd Copyright 1999 Acta Metallurgica Inc. Printed in the USA. All rights reserved. 1359-6462/99/\$ see front matter PII S1359-6462(99)00191-8

More information

### Deformation Twinning in Bulk Aluminum with Coarse Grains

Proceedings of the 12th International Conference on Aluminium Proceedings Alloys, of the September 12th International 5-9, 2010, Yokohama, Conference Japan on 2010 Aluminum The Japan Alloys, Institute

More information

### Chapter 10, Phase Transformations

Chapter Outline: Phase Transformations Heat Treatment (time and temperature) Microstructure Kinetics of phase transformations Homogeneous and heterogeneous nucleation Growth, rate of the phase transformation

More information

### Chapter 3 Crystal Interfaces and Microstructure

Chapter 3 Crystal Interfaces and Microstructure Interfacial free energy Solid / vapor interfaces Boundaries in single-phase solids Interphase interfaces in solids Interface migration Interfacial Free Energy

More information

### Chapter 3 Structure of Crystalline Solids

Chapter 3 Structure of Crystalline Solids Crystal Structures Points, Directions, and Planes Linear and Planar Densities X-ray Diffraction How do atoms assemble into solid structures? (for now, focus on

More information

### Mat E 272 Lectures 22-23: Introduction to Ceramic Materials

Mat E 272 Lectures 22-23: Introduction to Ceramic Materials November 26 & 28, 2001 Introduction: The primary emphasis of this class has previously been on the structure and properties of pure metals and

More information

### Diffusion in Solids. Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases?

Diffusion in Solids ISSUES TO ADDRESS... How does diffusion occur? Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases? How does diffusion depend

More information

### Stress Fields Around Dislocations

Stress Fields Around Dislocations The crystal lattice in the vicinity of a dislocation is distorted (or strained). The stresses that accompanied the strains can e calculated y elasticity theory eginning

More information

### SOLID-STATE STRUCTURE.. FUNDAMENTALS

SOLID-STATE STRUCTURE.. FUNDAMENTALS Metallic Elements & Sphere Packing, Unit Celis, Coordination Number, Ionic Structures Stoichiometry PRELAB ASSIGNMENT Properties of Shapes & Patterns following question

More information

### Introduction to Dislocations

Introduction to Dislocations This page intentionally left blank Introduction to Dislocations Fifth Edition D. Hull and D. J. acon Department of Engineering, Materials Science and Engineering, University

More information

### Phase Diagrams. Phases

Phase Diagrams Reading: Callister Ch. 10 What is a phase? What is the equilibrium i state t when different elements are mixed? What phase diagrams tell us. How phases evolve with temperature and composition

More information

### Kinematical theory of contrast

Kinematical theory of contrast Image interpretation in the EM the known distribution of the direct and/or diffracted beam on the lower surface of the crystal The image on the screen of an EM = the enlarged

More information

### Energy and Packing. Materials and Packing

Energy and Packing Non dense, random packing Energy typical neighbor bond length typical neighbor bond energy r Dense, regular packing Energy typical neighbor bond length typical neighbor bond energy r

More information

### Torsional properties of bamboo-like structured Cu nanowires. Haifei Zhan and Yuantong Gu *

Torsional properties of bamboo-like structured Cu nanowires Haifei Zhan and Yuantong Gu * School of Chemistry, Physics and Mechanical Engineering, Queensland University of Technology, Brisbane, QLD, 4001,

More information

### Ceramics are inorganic, non-metallic. Ceramics. Ceramics exhibit ionic, covalent bonding or a combination of the two (like in Al 2 O 3 )

What are Ceramics? CERAMIC MATERIALS Ceramics are inorganic, non-metallic and crystalline materials that are typically produced using clays and other minerals from the earth or chemically processed powders

More information

### Crystal Structure. Andrew R. Barron Carissa Smith. 1 Introduction. 2 Crystallography

OpenStax-CNX module: m16927 1 Crystal Structure Andrew R. Barron Carissa Smith This work is produced by OpenStax-CNX and licensed under the Creative Commons Attribution License 2.0 1 Introduction In any

More information

### TRANSITION BETWEEN LOW AND HIGH ANGLE GRAIN BOUNDARIES

TRANSITION BETWEEN LOW AND HIGH ANGLE GRAIN BOUNDARIES Myrjam Winning 1, Anthony D. Rollett 1 Institut für Metallkunde und Metallphysik, RWTH Aachen, 5056 Aachen, Germany Carnegie Mellon University, Pittsburgh

More information

### Tensile Testing. Objectives

Laboratory 3 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine to achieve the

More information

### Solute Drag on Perfect and Extended Dislocations

To appear in Philosophical Magazine Vol., No., Month XX, 7 Solute Drag on Perfect and Extended Dislocations R.B. Sills a,b and W. Cai a a Department of Mechanical Engineering, Stanford University, CA 9435,

More information

### MatCalc approach for the modelling of the vacancy concentration evolution

MatCalc approach for the modelling of the vacancy concentration evolution (MatCalc 6.00.0200) P. Warczok Outline Vacancy concentration Vacancies in solids - What is it all about? Influence on diffusion

More information

### Mobility laws in dislocation dynamics simulations

Materials Science and Engineering A 387 389 (2004) 277 281 Mobility laws in dislocation dynamics simulations Wei Cai, Vasily V. Bulatov Lawrence Livermore National Laboratory, University of California,

More information

### Creep and High Temperature Failure. Creep and High Temperature Failure. Creep Curve. Outline

Creep and High Temperature Failure Outline Creep and high temperature failure Creep testing Factors affecting creep Stress rupture life time behaviour Creep mechanisms Example Materials for high creep

More information

### Alloys and Solid Solutions

Alloys and Solid Solutions Chemistry 123 Spring 2008 Dr. Woodward Solutions Solid Solution 14 Carat Gold Liquid Solution Vodka Gaseous Solution Air Solution = A homogeneous mixture 1 Alloys An alloy is

More information

### Introduction to Dislocation Mechanics

Introduction to Dislocation Mechanics What is Dislocation Mechanics? (as meant here) The study of the stress state and deformation of continua whose elastic response is mediated by the nucleation, presence,

More information

### ENERGY AND PACKING. Chapter 3 CRYSTAL STRUCTURE & PROPERTIES MATERIALS AND PACKING METALLIC CRYSTALS ISSUES TO ADDRESS...

Chapter 3 CRYSTAL STRUCTURE & PROPERTIES ISSUES TO ADDRESS... 1. How do s assemble into solid structures? (For now, focus on metals) ENERGY AND PACKING non dense, random packing bond energy Energy bond

More information

### DOE FUNDAMENTALS HANDBOOK

DOE-HDBK-1017/1-93 JANUARY 1993 DOE FUNDAMENTALS HANDBOOK MATERIAL SCIENCE Volume 1 of 2 U.S. Department of Energy Washington, D.C. 20585 FSC-6910 Distribution Statement A. Approved for public release;

More information

### ORIENTATION DEPENDENCE OF DISLOCATION STRUCTURE EVOLUTION OF ALUMINUM ALLOYS IN 2-D AND 3-D COLIN CLARKE MERRIMAN

ORIENTATION DEPENDENCE OF DISLOCATION STRUCTURE EVOLUTION OF ALUMINUM ALLOYS IN 2-D AND 3-D By COLIN CLARKE MERRIMAN A thesis submitted in partial fulfillment of the requirements for the degree of: MASTER

More information

### Module 1. Principles of Physical Metallurgy: an introduction to the course content. Lecture 1

Module 1 Principles of Physical Metallurgy: an introduction to the course content Lecture 1 Principles of Physical Metallurgy: an introduction to the course content 1 Keywords: Cost of metals & materials,

More information

### Module #25. Martensitic Transformations and Strengthening

Module #25 Martensitic Transformations and Strengthening READING LIST DIETER: Ch. 6, pp. 226-228. Chapter 11 in Meyers & Chawla. Chapter 13 in P. Haasen, Physical Metallurgy, 3 rd Edition, Cambridge University

More information

### C&wsK 0! </-//</</ jy

QiSJRIittliCIt W litis, OSCUMEKT r UiUM*rE& ^7 C&wsK 0!

More information

### Titanium and titanium alloys. Josef Stráský

Titanium and titanium alloys Josef Stráský Lecture 2: Fundamentals of Ti alloys Polymorphism Alpha phase Beta phase Pure titanium Titanium alloys alloys alloys alloys Phase transformation β α phase Hardening

More information

### Materials Science Handbook: Volume 1 Structure and Properties of Metals 5 PDH / 5 CE Hours

Materials Science Handbook: Volume 1 Structure and Properties of Metals 5 PDH / 5 CE Hours DOE Fundamentals Handbook Material Science Volume 1 of 2 DOE-HDBK-1017/1-93 PDH Academy PO Box 449 Pewaukee, WI

More information